CO2 Corrosion Notes
Embed Size (px)
Transcript of CO2 Corrosion Notes
CO2 Information Carbon dioxide systems are one of the most common environments in the oil field industry where corrosion occurs. Carbon dioxide forms a weak acid known as carbonic acid (H2CO3) in water, a relatively slow reaction. However, CO2 corrosion rates are greater than the effect of carbonic acid alone. Cathodic depolarization may occur, and other attack mechanisms may also be at work. The presence of salts is relatively unimportant. Corrosion rates in a CO2 system can reach very high levels (thousands of mils per year), but it can be effectively inhibited. Velocity effects are very important in the CO2 system; turbulence is often a critical factor in pushing a sweet system into a corrosive regime. This is because it either prevents formation or removes a protective iron carbonate (siderite) scale. Conditions favoring the formation of the protective iron carbonate scale are elevated temperature, increased pH (bicarbonate waters) and lack of turbulence. Magnetite scales are also formed in CO2 systems, and corrosion product scales often consist of layers or mixtures of siderite and magnetite. The maximum concentration of dissolved CO2 in water is 800 ppm. When CO2 is present, the most common forms of corrosion include uniform corrosion, pitting corrosion, wormhole attack, galvanic ringworm corrosion, heat affected corrosion, mesa attack, raindrop corrosion, erosion corrosion, and corrosion fatigue. The presence of carbon dioxide usually means no H2 embrittlement. For more on the theory and mechanisms for each corrosion type, go to the theory pages CO2 corrosion products include iron carbonate (siderite, FeCO3), Iron oxide, and magnetite. Corrosion product colors may be green, tan, or brown to black. Top Where Found As stated before, CO2 corrosion is one of the most common environments where corrosion occurs, and exists almost everywhere. Areas where CO2 corrosion is most common include flowing wells, gas condensate wells, areas where water condenses, tanks filled with CO2, saturated produced water and flowlines, which are generally corroded at a slower rate because of lower temperatures and pressures. For more
information on specific equipment corrosion issues, refer to the equipment pages. CO2 corrosion is enhanced in the presence of both oxygen and organic acids, which can act to dissolve iron carbonate scale and prevent further scaling. Top Prevention / Mitigation To reduce or prevent corrosion in an CO2 environment: Drilling - pH control with caustic soda Producing wells - corrosion inhibitors Flowlines - continuous corrosion inhibitor injection Prediction of corrosion In sweet gas wells with a pH of 7 or less, a CO2 partial pressure of 30 psi usually indicates corrosion. a CO2 partial pressure of 7 - 30 psi may indicate corrosion. a CO2 partial pressure of 7 psi is usually considered non-corrosive. Top Pictures - Click on thumbnail to see larger picture
Pitting Corrosion showing wormhole attack pattern, where pits are interconnected.
Galvanic ringworm corrosion, often occurring four to six inches from the upset, where carbon particles have been spheroidized.
Heat-affected zone (HAZ) corrosion is a type of galvanic corrosion which occurs along a weld seam.
Raindrop attack occurs in gas condensate wells. In areas, water condenses on the metal surface, causing deep pits with tails.
CO2 corrosion in flowing environments
Mesa attack is a form of CO2 corrosion that occurs in flowing environments, and occurs where a protective iron carbonate coating is worn away in areas.
Erosion Corrosion, or flow-enhanced corrosion, usually occurs in areas where the diameter of the pipe or direction of flow is changing. Severe metal loss can quickly occur.
Corrosion due to fatigue occurs in areas of cyclic stresses. Here we see fatigue corrosion in a drill pipe.
asic Corrosion TheoryCorrosion is an electrochemical reaction composed of two half cell reactions, an anodic reaction and a cathodic reaction. The anodic reaction releases electrons, while the cathodic reaction consumes electrons. There are three common cathodic reactions, oxygen reduction (fast), hydrogen evolution from neutral water (slow), and hydrogen evolution from acid (fast).
The corrosion cell
The corrosion cell can be represented as follows:
Anodic reaction: M Mn+ + neM stands for a metal and n stands for the number of electrons that an atom of the metal will easily release. i.e. for iron and steel: Fe Fe2+ + 2eCathodic reactions: O2 + 4 H+ + 4e- 2H2O (oxygen reduction in acidic solution) 1/2 O2 + H2O + 2e- 2 OH- (oxygen reduction in neutral or basic solution) 2 H+ + 2e- H2 (hydrogen evolution from acidic solution) 2 H2O + 2e- H2 + 2 OH- (hydrogen evolution from neutral water) Each half-cell reaction has an electrical potential, known as the half-cell electrode potential. The anodic reaction potential, Ea , plus the cathodic reaction potential, Ec , adds up to E, the cell potential. If the overall cell potential is positive, the reaction will proceed spontaneously.
Every metal or alloy has a unique corrosion potential in a defined environment. When the reactants and products are at an arbitrarily defined standard state, the half-cell electrode potentials are designated Eo. These standard potentials are measured with respect to the standard hydrogen electrode (SHE). A listing of
standard half-cell electrode potentials is given in Table 1. Selected half-cell reduction potentials are given in Table 1. To determine oxidation potentials, reverse the direction of the arrow and reverse the sign of the standard potential. For a given cathodic reaction, those anodic (reversed) reactions below it in the table will go spontaneously, while those above it will not. Thus any metal below the hydrogen evolution reaction will corrode (oxidize) in acidic solutions. e.g., Cathodic reaction: 2H+ + 2e- H2 (hydrogen evolution) Two possible anodic reactions: Cu Cu2+ + 2e- (above cathodic rxn in table - will not corrode) Zn Zn2+ + 2e- (below cathodic rxn in table - spontaneous corrosion) Thus, in the presence of H+ ions, Zinc (Zn) will spontaneously corrode while copper (Cu) will not. Table 1. Standard Electromotive Force Potentials Cathodic Reactions Au3+ + 3e- Au O2 + 4H+ + 4e- 2H2O Pt2+ + 2e- Pt NO3- + 4H+ + 3e- NO + 2H2O Ag+ + e- Ag O2 + 2H2O + 4e- 4OHCu2+ + 2e- Cu 2H+ + 2e- H2 Pb2+ + 2e- Pb Sn2+ + 2e- Sn Ni2+ + 2e- Ni Co2+ + 2e- Co Cd2+ + 2e- Cd Fe2+ + 2e- Fe Cr3+ + 3e- Cr Zn2+ + 2e- Zn 2H2O + 2e- H2 + 2OHAl3+ + 3e- Al Mg2+ + 2e- Mg Na+ + e- Na K+ + e- K Standard Potential, eo (volts vs. SHE) +1.498 (Most Noble) +1.229 (in acidic solution) +1.118 +0.957 +0.799 +0.401 (in neutral or basic solution) +0.337 0.000 -0.126 -0.138 -0.250 -0.277 -0.403 -0.447 -0.744 -0.762 -0.828 (pH = 14) -1.662 -2.372 -2.71 -2.931 (Most Active)
Source: Handbook of Chemistry and Physics, 71st ed, CRC Press, 1991 Table 1 can be used to show that copper will corrode in nitric acid solutions (oxidizing) and aerated water. Similarly, aluminum (Al), magnesium (Mg), sodium (Na) and potassium (K) will react spontaneously with water in neutral or basic solutions.
Why corrosion cells formCorrosion cells are created on metal surfaces in contact with an electrolyte because of energy differences between the metal and the electrolyte. Different area on the metal surface could also have different potentials with respect to the electrolyte. These variations could be due to i) metallurgical factors, i.e., differences in their composition, microstructure, fabrication, and field installations, and ii) environmental factors. Carbon and low alloy steels are the most widely used material in the oilfield. Stainless steels (Fe-Cr-Ni), and nickel-base corrosion resistant alloys (CRA), such as Incoloys (Ni-Fe-Cr), Inconels (Ni-Cr), Hastelloys (Ni-Cr-Mo-Fe-Co) etc., are also used in highly corrosive environments. i) Metallurgical factors Steel is an alloy of iron (Fe) and carbon (C). Carbon is fairly soluble in liquid iron at steel making temperatures, however, it is practically insoluble in solid iron (0.02% at 723C), and trace at room temperature. Pure iron is soft and malleable; small amounts carbon and manganese are added to give steel its strength and toughness. Most of the carbon is oxidized during steelmaking. The residual carbon and postfabrication heat treatment determines the microstructure, therefore strength and hardness of steels. Carbon steels are then identified by their carbon contents, i.e., low-carbon or mild steel, medium carbon (0.2- 0.4 % C), high-carbon (up to 1% C) steels, and cast irons (>2 % C). American Iron and Steel Institute (AISI) designation 10xx series represent plain carbon steels, last two digits indicating the carbon content. For instance, AISI 1036 steel, commonly used in sucker rods, contain 0.36% carbon. Low alloy steels contain 1-3% alloying elements, such as chromium-molybdenum steels, 4140 (1% Cr-0.2% Mo-0.4% C), for improved strength and corrosion resistance. American Petroleum Institute (API) specifications also provide guidelines for strength and chemical composition of oilfield steels. During equilibrium solidification of steel, individual grains of almost pure iron (ferrite), and grains richer in iron carbide (cementite, Fe3C) within ferrite form. The lamellar carbide structure with ferrite is known as pearlite. If, however, steel is rapidly cooled to room temperature (quenched), carbon is retained in a highly strained matrix known as martensite. This structure is very hard and brittle and is not suitable for most engineering applications. The microstructure of fast cooled steels, for instance after welding or hot-rolling, are modified by reheating steels to a critical temperature range and controlled cooling, i.e., tempering, normalizing, and annealing.
The microstructure o